prev

next

out of 11

Published on

21-Jun-2016View

213Download

0

Transcript

The calculation of scalar transport during the injection molding of thermoset polymers

Foluso Ladeinde

SUNY at Stony Brook, Stony Brook, NY, USA

Hasan U. Akay

Technalysis Incorporated, Indianapolis, IN, USA

In this paper we present a numerical scheme for the calculation of the equation governing the advection of scalars such as temperature T and cure tl during the injection mold filling of thermoset polymers. A jinite-element line method is presented, with variations intended to cover a variety of processing conditions. Sample calculations are presented for the Garcia problem and the encapsulation of a Motorola computer chip. We also share our experience with some of the peculiar numerical difficulties associated with the simulation of injection molding for realistic systems. Some of these are related to mesh quality, time step size selection, and (numerical) degeneracy that could result from some otherwise physical material models. The foregoing are issues that have not received a great deal of attention in the literature.

Keywords: transport, injection molding, thermoset polymers

1. Introduction

The process of injection molding of polymers seems to have benefited greatly from emerging computer technol- ogy. For example, with commercially available computer codes such as PLASTEC,' the filling simulation could predict short shots, weld lines, air trapping, overheating, the number of gates and their locations for optimum design, balancing of runners, optimization of injection pressure and clamp force requirements, calculation of pressures, temperatures, shear rate, shear stress, velocity distribution, etc. Further, postfilling processes (packing, in the case of thermoplastics) can also be simulated to provide part shrinkage and the initial state of stress (needed for subsequent structural analysis of the part).

The simulations involve the solution of the momentum equations and the transport equations for one or more scalars (depending on whether the polymer is a thermoplastic or a thermoset). For thermoplastics, simulation complications include: (a) the need for an accurate non-Newtonian characterization of the polymer melt as it goes through the molding process-viscosity as a function of shear rate, temperature, and sometimes pressure, (b) complicated geometry-thin parts arbitarily oriented in three-dimensional space which, sometimes,

a Also at Indiana University-Purdue University, Indianapolis, IN, USA

Address reprint requests to Dr. Ladeinde at SUNY at Stony Brook, Stony Brook, NY 11794, USA,

Received 1 March 1993; revised 22 October 1993; accepted 29 November 1993

are combined with full three-dimensional parts, (c) moving fluid front, (d) fountain flow phenomenon at the front and, finally, (e) fiber orientation, as in Reifschneider, et al. Some examples of numerical simulation of injection molding include Broyer et al., Hieber and Shen3 Kamal et a1.,4 Wang et a1.,5 Ladeinde et a1.,6 and Subbiah et a1.7

Most of the computer simulation capabilities men- tioned in the first paragraph have been applied to thermoplastics and, to a lesser extent, to thermosetting polymers. However, we know that thermosetting polymers are the natural choice in applications where heat resistance is needed, an example being the use of epoxy molding compound (EMC) for the encapsulation of computer chips (to protect the delicate metallic layout from the heat that is generated). Thermosets present additional difficulties for simulation, including (a) the need to model the degree of cure (to be defined later in this paper), (b) a viscosity model that must now incorporate the effect of the degree of cure, and (c) the more significant effect of fountain flow on cure development, this being a consequence of the absence of dissipative effects, particularly at the top/bottom walls of the mold. There have been previous studies on computer simulation of thermoset polymers, these being exemplified by the works of Gonzalez et al.,* Shen, Garcia, aLI

Garcia et al., Turng et al., and Nguyen et

This paper focuses on thermosets, the filling of which involves the flow of a reactive mixture into molds. The viscosity of the reactants is initially low, to promote mixing and permit the filling of larger parts; but the

0 1994 Butterworth-Heinemann Appl. Math. Modelling, 1994, Vol. 18, June 347

Scalar transport during injection molding of polymers: F. Ladeinde and H. U. Akay

viscosity increases and the mixture ultimately gels and solidifies as a result of chemical cross-linkage or phase separation. For this kind of process, an optimum filling rate must be used, which should be slow enough to allow uniform (laminar) filling, but sufficiently high to prevent premature gelling. (In fact, EMC is the preferred material for microelectronic encapsulation because of its low initial viscosity, which allows it to flow over delicate lead frame and wire bonds without causing a large deformation, and its ability to undergo an additional (polymerization) reaction (during filling and postfilling), to acquire the mechanical and thermal properties that protect the electronic part from the environment.) We have observed in our work that the filling rate has a serious consequence for numerical procedures, one that is complicated by the moving boundary.

Most injection molding processes involve low Reynolds number and thin-walled parts in which the lateral dimensions (x, y) are much larger than the local thickness (z). Thus, the pressure is assumed constant along z and the Hele-Shaw approach is invoked, leading to the replacement of the momentum equations by a Poisson equation for pressure (RichardsonI and Hieber and Shenj). The equation, which is locally two- dimensional (in the plane of the part), is then solved, usually with the finite-element or finite-difference method. To advance the melt front, most people use the control volume approach in Wang et a1.5

coordinate directions and in a manner that obviates the foregoing difficulties. For example, we present variations of the scheme that allow the use of small or large time step sizes, as demanded by the filling rate. The usefulness of this capability will become more apparent when we discuss the crucial issue of time step size selection. Because we use the finite-element method in all three coordinate directions, we inherit the simplicity of applying complicated boundary conditions and arbitrary mesh grading in all coordinate directions. We will share our experience with some of the general difficulties associated with the simulation of injection molding for realistic systems. Some of these are related to mesh quality, time step size selection, and the (numerical) degeneracy that could result from some otherwise physical material models. These issues have not received much attention in the literature, leaving the reader (or a code-user) with the impression of robust and trouble-free calculations.

The mathematical formulation is presented in Section two, and the viscosity models of interest are discussed in Section three. Section four details the numerical procedure; in Section five, we discuss code validation. Concluding remarks are presented in Section six. An appendix is provided in which the elements of certain matrices are defined.

2. Mathematical formulation The pressure (melt front advancement) part of

injection molding simulation is cheap compared with the calculation of the transport of temperature T or the cure tl. Some reasons for this include the presence of nonlinear, nonsymmetric convective operators in the scalar transport equations, the high P&let number, the need for an accurate time integration, and the requirement for a full three-dimensional calculation in thin-walled geometries that are arbitrarily oriented in a three-dimensional space. Moreover, as discussed in Ladeinde et a1.,6 direct methods or fully explicit formulations are not desirable.

2.1 Governing equations

This paper focuses on the filling stage of the injection molding of thermoset polymers in three-dimensional thin parts. The Eulerian approach to the calculation of both T and c1 is presented, for which the governing equations are

v.svp=o (1)

aT aT +Udx+u- ay

$L:2T a9

I ,:r \ ,

We are aware of two main approaches for calculating temperature (and that are also applicable to the equation for cure). The first is ad hoc and involves the assumption of a profile across the thickness, without solving the conservative equations. Such simplicity was necessary decades ago when computing was very primitive. For obvious reasons, this procedure is prone to errors, and we feel it should be discontinued. The second approach used to calculate temperature combines a finite difference in the thickness direction with a finite-element procedure that is used to solve the pressure equation. Thus, this is a hybrid approach. In an implementation of this approach,3,5 terms of the temperature equation (such as ~?~T/az~ or u. VT) are defined as element quantities, and element contribution to a node is assumed to depend on the volume of the element. The procedure is tedious and does not appear flexible in terms of providing variations that could be explored to optimize the calculations for a variety of processing conditions.

+ $ Qnl+ vi* (2) ac( aa au da z+ux+v-==

ay dt (3)

Above, S is the fluidity, which is inversely propor- tional to melt viscosity, p is the pressure, p is the melt density, C, is the specific heat at constant pressure, T is temperature, and t is time. We also have k, which is the thermal conductivity of the melt; Q, is heat generation from the exothermic cure reaction, ye is viscosity, i is strain rate, (x, y, z) are the spatial coordinates, and (u, v) are the velocity components in the local (x, y) directions. LX is the degree of cure, defined as the ratio of the heat already released at time t under isothermal conditions, to the total heat that is releasable if the reaction is allowed to continue indefinitely, under the same conditions.

A contribution of this work is the presentation of a Two models for dccldt have been used in our work. The procedure that uses the finite-element method in all three first (Model 1) has been suggested by Garcia et al. and

348 Appl. Math. Modelling, 1994, Vol. 18, June

Scalar transport during injection molding of polymers: F, Ladeinde and H. U. Akay

is given by

dcc A

z = c, exp (4)

The second model (Model 2) is more common and has been shown to work very well. It is due to Kamal and Sourour and has the form:

da z = (K, + K2cP)(l - c)m2

where

Ki = K,(T) = a, exp( -EJT), i = 1,2 (6)

In these models, A, C,, E, Rgas, m, K,, K,, a,, a2, E,, E,, m,, and m2 are model constants. Model 1 can be expressed in terms of Model 2 as shown in Table 1. Also shown in Table 1 are the input values used in the present work to validate the proposed solution method and the equivalence between the heat of reaction in the two models.

2.2 Velocities and fluidity

The fluidity S is defined as

s= s b34 ~ d4 0 Y(%Y, 4) for planar parts or,

for pipes/ducts. (For noncircular pipes/ducts R rep- resents the equivalent radius, which is determined to give the same linear velocity as a circular pipe of radius R.) The velocities are

Above, (p is the vertical distance normalized by local (half gap) thickness, b. Consistent with the procedure used to obtain equation (l), we can define depth-averaged velocities:

80 _ ap S u= -xb)= _ayb

Table 1. Equivalence of parameters for cure models 1 and 2

For the thin geometries considered the strain rate can be written as

+[(~~+(@)2]1:2, 20 for planar parts, whereas for ducts we approximate +j by

dr

(uaxial is the velocity component in the axial direction of pipe.) Finally, conduction in the lateral plane (shown with underbrace in equation (2)) is very small for most applications and could be neglected in the equations. Also, neglecting them is consistent with the Hele-Shaw approach used to obtain the flow equation. (An adiabatic condition must be specified at surfaces where the conduction terms are neglected.) However, we retain both capabilities (Dirichlet and adiabatic), because our procedure can be applied to regular, nonthin parts, as we show later in the discussion of code validation.

2.3 Boundary conditions

The boundary conditions for pressure are: At sidewalls and inserts we use dp/an = 0, at free surface p = 0, and at cavity inlet we specify either p = p(t) or Q = Q(t), where Q = 2 Ic - SVp. ndC. For temperature, we have T,(x, y, z; t) at the top wall, aT/an = 0 at midplane, T = T,,ject at cavity inlet, and T = Tide or aTJan = 0 at the side walls. The boundary conditions for the degree of cure are aa /an = 0 at the top, &/dn = 0 at midplane, IX = uinject at cavity inlet, and &x/an = 0 at the side walls. The temperature and the degree of cure at the free surface are found by a fountain flow model that corresponds to the simplified front in Garcia et al. with the understanding that a more accurate model is required for fast filling. A schematic of the various boundary conditions for pressure and temperature is shown in Figure I.

3. Viscosity models

The applications require proper viscosity characteriza- tion for the melt, which usually implies dependence on strain rate, temperature, cure rate, and sometimes, pressure. Some materials/processes do not require more than the power law type models, whereas the relaxational feature of models such as the modified Cross are needed in many cases. Three viscosity models are used in our work, the first of which was introduced

Parameter Model 1 Model 2 Input value Unit

1 -

2 m

3 AC;- 4 5

E/&as -

6 -

Heat of reaction Cc&+,

0.0 2.0

2.545 x IO 6.399 x lo3

0.0 0.0 2.3208 x IO9

1 /set K 1 fsec K eras/cm3

Awl. Math. Modelling, 1994, Vol. 18, June 349

Scalar transport during injection molding of polymers: F. Ladeinde and H. U. Akay

Mold temperature or heat flux on the surfaGO

Speclfled side wall 4 Flowrate or pressura temperature or heat flux (time-dependent)

Figure 1. Schematic of the various boundary conditions for pressure and temperature.

by Castro and Macosko16 and has the form:

Here, A,, E,, R,, ugel, a, and b are the parameters of the model. The second viscosity that we have incorporated into our code is based on the modified Cross model:

rlo(T, PI tl

[ 1

a+ba

= 1 + G2(~0j)n-1 gel

a,,, - M

The (additional) parameters qO, G,, and n appear in this model. Finally, we have used a model from Garcia:

1 I[ 1 o+ba

q = A,exp agel

C + d(T - ZJ ~~~~ - LX

C, d, and T, are model parameters; T, is the glass transition temperature, for which the form quoted in Sheng has been used.

4. Numerical procedure

4.1 The lay-fiat transformation

Equations (1)+3) are in terms of some global Cartesian coordinates. However, to solve these equations for a complex (thin) part with arbitrary orientations in space, each element is transformed so that the part as a whole is laid-flat, to reconcile coordinates (...